Aluminium gallium antimonide

Aluminium gallium antimonide, also known as gallium aluminium antimonide or AlGaSb (AlxGa1-xSb), is a ternary III-V semiconductor compound. The alloy can contain any ratio between aluminium and gallium; that is, x in the formula can continuously take on any value between 0 and 1. AlGaSb refers generally to any composition of the alloy.

The bandgap and lattice constant of AlGaSb alloys are between those of pure AlSb (a = 0.614 nm, Eg = 1.62 eV) and GaSb (a = 0.610 nm, Eg = 0.73 eV).[1] At an intermediate composition, the bandgap transitions from an indirect gap, like that of pure AlSb, to a direct gap, like that of pure GaSb. Different values of the composition at which this transition occurs have been reported over time, both from computational and experimental studies, with reported values ranging from x = 0.23 to x = 0.41.[1][2][3]

## Preparation[edit]

AlGaSb films have been grown by molecular beam epitaxy, chemical beam epitaxy[4] and liquid phase epitaxy[5] on gallium arsenide and gallium antimonide substrates. It is often incorporated into layered heterostructures with other III-V compounds.

## Applications[edit]

AlGaSb has been incorporated into devices such as heterojunction bipolar and high-electron-mobility transistors[6][7][8], resonant-tunneling diodes[9], solar cells[10], short-wave infrared lasers[11], and a novel infrared light modulator[12]. It is sometimes selected as an interlayer or buffer layer in studies of GaSb and InAs quantum wells.

Al-rich AlGaSb is sometimes selected over AlSb in heterostructures for being more chemically stable and resistant to oxidation than pure AlSb.[6][7]

## References[edit]

1. ^ a b Vurgaftman, I., Meyer, J. R., Ram-Mohan, L. R. (2001). "Band parameters for III–V compound semiconductors and their alloys". Journal of Applied Physics. 89 (11): 5815–5875. doi:10.1063/1.1368156.
2. ^ Wang, F., Jia, Y., Li, S.-F., Sun, Q. (2009). "First-principles calculation of the 6.1 Å family bowing parameters and band offsets". Journal of Applied Physics. 105 (4): 043101. doi:10.1063/1.3072688.
3. ^ Mathieu, H., Auvergne, D., Merle, P., Rustagi, K. C. (1975). "Electronic energy levels in Ga1−xAlxSb alloys". Physical Review B. 12 (12): 5846–5852. doi:10.1103/PhysRevB.12.5846.
4. ^ Okuno, Y., Asahi, H., Kaneko, T., Itani, Y., Asami, K., Gonda, S. (1991). "MOMBE growth of AlGaSb". Journal of Crystal Growth. 115 (1–4): 236–240. doi:10.1016/0022-0248(91)90745-Q.
5. ^ Wada, T., Kubota, K., Ikoma, T. (1984). "Liquid phase epitaxial growth of AlGaSb". Journal of Crystal Growth. 66 (3): 493–500. doi:10.1016/0022-0248(84)90147-7.
6. ^ a b Bennett, B. R., Khan, S. A., Boos, J. B., Papanicolaou, N. A., Kuznetsov, V. V. (2010). "AlGaSb Buffer Layers for Sb-Based Transistors". Journal of Electronic Materials. 39 (10): 2196–2202. doi:10.1007/s11664-010-1295-0.
7. ^ a b Bennett, B. R., Boos, J. B., Ancona, M. G., Papanicolaou, N. A., Cooke, G. A., Kheyrandish, H. (2007). "InAlSb/InAs/AlGaSb Quantum Well Heterostructures for High-Electron-Mobility Transistors". Journal of Electronic Materials. 36 (2): 99–104. doi:10.1007/s11664-006-0057-5.
8. ^ Furukawa, A., Mizuta, M. (1988). "Heterojunction bipolar transistor utilising AlGaSb/GaSb alloy system". Electronics Letters. 24 (22): 1378. doi:10.1049/el:19880943.
9. ^ Magno, R., Bracker, A. S., Bennett, B. R. (2001). "Resonant interband tunnel diodes with AlGaSb barriers". Journal of Applied Physics. 89 (10): 5791–5793. doi:10.1063/1.1365940.
10. ^ Vadiee, E., Renteria, E., Zhang, C., Williams, J. J., Mansoori, A., Addamane, S., Balakrishnan, G., Honsberg, C. B. (2017). "AlGaSb-Based Solar Cells Grown on GaAs: Structural Investigation and Device Performance". IEEE Journal of Photovoltaics. 7 (6): 1795–1801. doi:10.1109/JPHOTOV.2017.2756056.
11. ^ Wang, C. A., Jensen, K. F., Jones, A. C., Choi, H. K. (1996). "n -AlGaSb and GaSb/AlGaSb double-heterostructure lasers grown by organometallic vapor phase epitaxy". Applied Physics Letters. 68 (3): 400–402. doi:10.1063/1.116698.
12. ^ Xie, H., Wang, W. I. (1993). "Normal incidence infrared modulator using direct–indirect transitions in GaSb quantum wells". Applied Physics Letters. 63 (6): 776–778. doi:10.1063/1.109904.

* v
* t
* e

Aluminium compounds

Al(I)|

* AlBr
* AlCl
* AlF
* AlI
* Al2O
* AlOH

| Organoaluminium(I) compounds|

Al(C5(CH3)5)

|

Al(II)|

* AlB2
* AlB12
* AlO

Al(III)|

* AlAs
* Al(BH4)3
* AlBr3
* Al(CN)3
* AlCl3
* AlF3
* AlH3
* AlI3
* AlN
* Al(NO3)3
* Al2(CO3)3
* Al(OH)3
* Al(OH)2OAc
* Al(OH)(OAc)2
* Al(OAc)3
* Al2SO4(OAc)4
* AlP
* AlPO4
* AlSb
* Al(C5H7O2)3
* Al(MnO4)3
* Al2(MoO4)3
* Al2O3
* Al2S3
* Al2(SO4)3
* Al2Se3
* Al2Te3
* Al2SiO5
* AlAsO4
* Al4C3
* AlOHO
* Al(OH)2CO2C17H5
* NaAlH2(OC2H4OCH3)2
* LiAlH2(OC2H4OCH3)2
* K2Al2B2O7

| Alums|

* (NH4)Al(SO4)2
* KAl(SO4)2
* NaAl(SO4)2

|

Organoaluminium(III) compounds|

* Al(C3H5O3)3
* C
36H
69AlO

* (Al(CH3)3)2
* (Al(C2H5)3)2
* Al(CH2CH(CH3)2)3
* Al(C2H5)2Cl
* Al(C2H5)2CN
* Al(CH2CH(CH3)2)2H
* Al(C2H5)2Cl2C2H5Cl
* Ti(C5H5)2CH2ClAl(CH3)2

* v
* t
* e

Gallium compounds

Gallium(-V)|

* Mg5Ga2

Gallium(I)|

* Ga2O
* GaCl
* GaBr
* GaI

Gallium(II)|

* GaS
* GaSe
* GaTe

Gallium(I,III)|

* GaCl2

Gallium(III)|

* GaAs
* GaH3
* Ga2H6
* GaBr3
* GaCl3
* GaF3
* GaI3
* GaN
* Ga(OH)3
* Ga(CN)3
* Ga(NO3)3
* Ga2(SO4)3
* GaPO4
* GaP
* GaSb
* Ga2O3
* Ga2S3
* Ga2Se3
* Ga(CH3COO)3
* Ga2Te3

| Organogallium(III) compounds|

* Ga(C5H7O2)3
* Ga(CH3)3
* Ga(C2H5)3

|

* v
* t
* e

Antimony compounds

Antimonides|

* AlSb
* Bi1-xSbx
* GaSb
* InSb
* PrSb
* YSb
* ZnSb

Sb(III)|

* SbBr3
* Sb(C2H3O2)3
* SbCl3
* SbF3
* Sb4O4(OH)2(NO3)2
* SbH3
* SbI3
* SbN3
* Sb2O3
* Sb2S3
* Sb2(SO4)3
* Sb2Se3
* Sb2Te3

| Organoantimony(III) compounds|

* Sb(CH3)3
* Sb(C6H5)3

|

Sb(III,V)|

* Sb2O4

Sb(V)|

* SbCl5
* SbF5
* Sb2O5
* Sb2S5

| Organoantimony(V) compounds|

* Sb(CH3)5
* Sb(C6H5)5

|

*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template